**Piezo-optic tensor of crystals from quantum-mechanical calculations**

A. Erba,1,a)_{M. T. Ruggiero,}2

_{T. M. Korter,}2

_{and R. Dovesi}1

1_{Dipartimento di Chimica, Università di Torino and NIS, Nanostructured Interfaces and Surfaces,}
Centre of Excellence, Via Giuria 5, 10125 Torino, Italy

2_{Department of Chemistry, Syracuse University, 1-014 Center for Science and Technology,}
Syracuse, New York 13244-4100, USA

(Received 3 September 2015; accepted 29 September 2015; published online 12 October 2015) An automated computational strategy is devised for the ab initio determination of the full fourth-rank piezo-optic tensor of crystals belonging to any space group of symmetry. Elastic sti↵ness and compliance constants are obtained as numerical first derivatives of analytical energy gradients with respect to the strain and photo-elastic constants as numerical derivatives of analytical dielectric tensor components, which are in turn computed through a Coupled-Perturbed-Hartree-Fock/Kohn-Sham approach, with respect to the strain. Both point and translation symmetries are exploited at all steps of the calculation, within the framework of periodic boundary conditions. The scheme is applied to the determination of the full set of ten symmetry-independent piezo-optic constants of calcium tungstate CaWO4, which have recently been experimentally reconstructed. Present calculations unambiguously determine the absolute sign (positive) of the ⇡61 constant, confirm the reliability of 6 out of 10 experimentally determined constants and provide new, more accurate values for the remaining 4 constants. C 2015 AIP Publishing LLC. [http://dx.doi.org/10.1063/1.4932973]

**I. INTRODUCTION**

Several optical properties of anisotropic media are related
to birefringence or double refraction. It is indeed well-known
that two plane polarized electro-magnetic waves, with two
distinct velocities v, may in general be propagated through
a crystal with the same propagation direction. The c/v ratio
for each wave (c being the speed of light) is referred to as
the refractive index for that wave and can be derived for any
propagation direction from the so-called optical indicatrix: an
ellipsoid oriented along the principal axes of the dielectric
tensor ✏ and whose semi-axes give the principal refractive
indices of the system.1_{It follows that any change in the shape,}
size, and orientation of the indicatrix results in the
modifi-cation/modulation of the optical properties of a crystal. Such
changes can be induced by electric fields, strains and stresses
giving rise to the electro-optic, elasto-optic (i.e., photo-elastic),
and piezo-optic e↵ects, respectively.

In particular, the piezo-optic e↵ect (measuring the
vari-ation of the dielectric tensor components as induced by an
applied stress) has proven to be an e↵ective tool for
mapp-ing 2D and 3D mechanical stresses through stress
tensor-field tomography.2,3_{Furthermore, such an e↵ect is extremely}
relevant to the field of optoelectronics where the search for
highly efficient electro-optic and piezo-optic materials is
expe-riencing a great interest in recent years due to their
applica-tions as photo-elastic modulators of light polarization and as
components of many devices related to acousto-optic light
modulators, deflectors, tunable spectral filters, etc.4–11 _{The}
piezo-optic and photo-elastic responses of a crystal are quite
anisotropic even for high-symmetry systems. In order to
accu-rately optimize the orientation of a crystal, which maximizes
a)_{Electronic mail: alessandro.erba@unito.it}

the efficiency of the acousto-optic transformation, absolute values, and signs of all non-zero elements of the fourth-rank elastic C, compliance S, photo-elasticp, and piezo-optic ⇡ tensors have to be determined, which is not a trivial task (see below), especially for low-symmetry crystals.10,12,13

From an experimental point of view, photo-elastic
con-stants could be measured through acousto-optic methods.
Within the phenomenological theory of Brillouin scattering,
for instance, photo-elastic constants are given in terms of
the intensities of Brillouin components.14,15 _{Acousto-optic}
methods, however, are unable to uniquely determine all signs
of the photo-elastic constants, particularly so for
low-symme-try crystals.4,12 _{The full set of independent piezo-optic }
con-stants can be measured for crystals of any symmetry via the
combination of optical interferometry and polarization-optical
techniques (once the elastic compliances are known).12,16–18
Still, this approach requires a large number of measurements
to be performed on a large number of crystalline samples
(properly cut to specific orientations). In their fundamental
work of 2005, Andrushchak et al.12_{derived the minimum set of}
samples and measurements necessary to determine the whole
piezo-optic tensor for all crystal families: 57 measurements
on 16 samples are required to determine the 36
indepen-dent components of a triclinic crystal, 29 measurements on 8
samples for the 20 independent components of a monoclinic
crystal, 14 measurements on 6 samples for the 10 independent
components of tetragonal crystals belonging to the 4, 4 or 4/m
classes, just to name a few. Even small errors in the sample
cut preparation or in the alignment of the whole optical setup
may result in large errors in the piezo-optic constants
deter-mination (see the detailed analysis on the possible sources of
inaccuracies given by Krupych et al. in Ref.16). Furthermore,
the interferometric method is known to provide a somewhat
poor description of so-called rotating piezo-optical constants

(those which correspond to a rotation of the optical indicatrix under mechanical stress); a conoscopic method has recently been devised to determine such constants more accurately.19

In this paper we present a general, fully automated scheme
for the theoretical ab initio calculation of the fourth-rank
piezo-optic tensor ⇡ of crystals belonging to any space group
symmetry, which requires the simultaneous determination of
the elastic sti↵ness and compliance tensors and of the
photo-elastic tensor. The scheme adopts periodic-boundary
condi-tions, fully exploits both point and translational symmetries
at all steps,20–23 _{is based on the evaluation of analytical }
en-ergy gradients with respect to both atomic coordinates and
lattice parameters24–27 _{and utilizes the analytical }
Coupled-Perturbed-Hartree-Fock/Kohn-Sham (CPHF/KS) method to
compute static and electric field frequency-dependent optical
(i.e., dielectric) properties of crystals.28–30 _{We have }
imple-mented the present scheme into a development version of the
public Crystal14 program,31,32_{taking advantage of the many}
recent developments made to the algorithms for the evaluation
of strain-related tensorial properties (elastic, piezoelectric,
photo-elastic) of crystals.33–38

The proposed scheme is first described in detail and then
applied to the determination of the piezo-optic tensor of
tetrag-onal calcium tungstate, CaWO4, which belongs to the scheelite
family of minerals. This is a promising material for
acousto-optic modulators and its full set of piezo-acousto-optic (and
photo-elastic) constants has been experimentally determined only
quite recently.13,17–19 _{An explicit investigation is performed}
on the e↵ect of adopting several functionals of density
func-tional theory (DFT) belonging to three rungs of the so-called
“Jacob’s ladder”39_{(namely, a local-density approximation, a}
generalized-gradient approximation, and a couple of global
hybrids), and on the electric field frequency-dependence of
all computed dielectric, piezo-optic, and photo-elastic
prop-erties. Our calculations allow us to confirm the experimentally
measured values of a sub-set of the 10 independent piezo-optic
and photo-elastic constants of CaWO4and, on the contrary, to
point-out large discrepancies in the determination of the others
and to provide a complete description of the anisotropic
stress-optical response of this crystal.

**II. THEORY AND METHODS**

**A. Stress-related tensorial properties of crystals**
**and their symmetry features**

The stress-strain relation for an anisotropic crystal is given by the generalized Hooke’s law,

ij=Cijkl⌘kl, (1)

which relates the second-rank stress tensor to the second-rank pure strain tensor ⌘ through the 81 elastic sti↵ness con-stants Cijklthat constitute the fourth-rank elastic tensor C. In the above expression, i, j, k,l are Cartesian indices. As both and ⌘ are symmetric tensors, the number of their independent components reduces from 9 to 6, and those of C accordingly from 81 to 36. As a consequence, Voigt’s notation can be used, which introduces a mapping between pairs of Cartesian indices and Voigt’s indices running from 1 to 6: v, u = 1, . . . ,6 where

1 = xx, 2 = y y, 3 = zz, 4 = yz, 5 = xz and 6 = x y:1

v=Cvu⌘u and ⌘v=Svu u, (2)

where the fourth-rank elastic tensor has been given a 6 ⇥ 6
matrix representation and where S = C 1 _{represents the }
so-called elastic compliance tensor. To second-order in the strain,
the elastic constants can be defined as second energy density
derivatives with respect to pairs of strains,

Cvu= 1 V @2E @⌘v@⌘u ! , (3)

being V the volume of the crystal cell. From Equation(3),
the equivalence Cvu⌘ Cuvis evident, which makes the 6 ⇥ 6 C
matrix symmetric and reduces the number of its independent
components to 21. Neumann’s principle, which states that any
physical property of a crystal must exhibit at least the same
point-symmetry of the crystal, can be exploited to further
reduce the number of independent components by imposing
the invariance (CR_{= C}_{) of the fourth-rank elastic tensor to the}
action of any point-symmetry operator ˆR of the point-group to
which the crystal belongs,

CR

ijkl=riprjqrksrltCpqst, (4) where r is the 3 ⇥ 3 Cartesian matrix representation of the sym-metry operator ˆR and Einstein’s notation is used according to which repeated indices are meant to be summed. By imposing the invariance of C with respect to all the symmetry operators of the 4/m class of the tetragonal crystal system to which CaWO4 belongs, the following shape of the elastic tensor is obtained, for instance,

C = *. .. .. .. .. .. , C11 C12 C13 0 0 C16 C12 C11 C13 0 0 C16 C13 C13 C33 0 0 0 0 0 0 C44 0 0 0 0 0 0 C44 0 C16 C16 0 0 0 C66 +/ // // // // // -. (5)

In the present implementation, elastic constants in Equation(3) are computed as numerical first-derivatives of analytical en-ergy gradients.33,40

The variation of the components of the inverse dielectric
tensor ✏ 1_{as induced by strain is given by the strain-optical}
coefficients (i.e., elements of the fourth-rank Pockels’
elasto-optic or photo-elastic tensorp),

✏_{ij}1=pijkl⌘kl. (6)

As both the inverse dielectric tensor ✏ 1_{and the pure strain}
tensor ⌘ are symmetric, Voigt’s notation can be adopted also in
this case so that the photo-elastic tensorp can be given a 6 ⇥ 6
matrix representation as for the elastic tensor. Photo-elastic
constants can then be derived according to

pvu=@✏ 1 v @⌘u

, (7)

where, in the present scheme, the derivative with respect to the strain is evaluated numerically while the dielectric tensor (✏ =1 + 4⇡↵/V) analytically from the polarizability ↵ deter-mined through the CPHF/KS method (for a closed-shell

system),31
↵ij= 2
nk
BZ
X
k
< Tr Ck†⌦k,iCkUk, jn , (8)
where nkis the number ofk points in the first Brillouin Zone
(BZ) and n is the diagonal occupation matrix whose elements
are 2 for occupied orbitals and 0 otherwise. Here Uk, j _{is an}
anti-Hermitian block o↵-diagonal matrix that relates the
unper-turbed coefficient matrix Ck_{, to the corresponding first-order}
perturbed matrix, Ck, j_{⌘ C}k_{U}k, j_{, which gives the linear }
(first-order) response to the electric field perturbation represented
by the matrix ⌦k,i_{. The o↵-diagonal blocks of}_{U}k, j_{depend not}
only on ⌦k, j_{but also on the first-order perturbed density matrix}
(through the two-electron terms in the Hamiltonian) which, in
turn, depends uponUk, j_{. Hence, a self-consistent solution of}
the CPHF/KS equations is required.

As recalled in the introduction, the dielectric tensor ✏ determines the optical indicatrix of the crystal. For cubic crys-tals the indicatrix is a sphere. For hexagonal, tetragonal (as CaWO4), and trigonal crystals (optically uniaxial), the indica-trix is an ellipsoid of revolution about the principal symmetry axis of the system (also called optic axis). The section of the in-dicatrix perpendicular to the optic axis is a circle whose radius no is the ordinary refractive index of the system while the section perpendicular to any other direction is an ellipse whose semi-axes are no and ne, the latter being the extraordinary refractive index. Calcium tungstate is said to be an optically positive crystal as ne>no. The birefringence of a material can be defined as = ne no.

Given stress-strain relation (2), the fourth-rank piezo-optic tensor ⇡ (whose elements are the stress-piezo-optical coeffi-cients ⇡vu) can be obtained from the photo-elasticp and elastic Cones as1

⇡ =p S and conversely p = ⇡ C. (9)

At variance with the elastic C and compliance S tensors,p and
⇡are not symmetric (i.e., in general pvu, puvand ⇡vu, ⇡uv).
It follows that the number of symmetry-independent
compo-nents to be determined for the stress-optical and strain-optical
tensors is generally larger than for the elastic tensors. The
invariance of the piezo-optic tensor with respect to all the
point-symmetry operators ˆR of the crystal has to be imposed
(⇡R_{=}_{⇡}_{) without the constraint of being symmetric,}

⇡_{ijkl}R =riprjqrksrlt⇡pqst. (10)
For instance, a triclinic crystal has 36 independent piezo-optic
coefficients, with the number of unique values decreasing with
increasing symmetry. In the case of CaWO4(tetragonal 4/m),
the shape of the piezo-optic tensor is

⇡ = *. .. .. .. .. .. , ⇡11 ⇡12 ⇡13 0 0 ⇡16 ⇡12 ⇡11 ⇡13 0 0 ⇡16 ⇡31 ⇡31 ⇡33 0 0 0 0 0 0 ⇡44 ⇡45 0 0 0 0 ⇡45 ⇡44 0 ⇡61 ⇡61 0 0 0 ⇡66 +/ // // // // // -. (11)

The piezo-optic coefficients ⇡vu where both v, u = 1,2,3
describe the connection between the principal refractive
indices and the normal stresses and are referred to as principal
coefficients. Coefficients ⇡vuwhere v = 1,2,3 and u = 4,5,6
relate the principal refractive indices to shear stresses and are
called shifting coefficients. Piezo-optic coefficients where v
=4,5,6 correspond to the rotation of the optical indicatrix and
are called rotating or rotating-shifting coefficients depending
on whether u = 1,2,3 or u = 4,5,6, respectively.3_{Photo-elastic}
constants pvu are dimensionless while piezo-optic ⇡vu ones
are generally expressed in units of Brewsters, where 1 Br
=10 12Pa 1=1 TPa 1.

**B. The automated algorithm**

One of the specific features of the present scheme for
the evaluation of the piezo-optic fourth-rank tensor of
crys-tals of any symmetry is its fully automated character, which
requires a “one-shot” calculation of elastic, dielectric and
photo-elastic constants, and their combination. Such a scheme
involves the efficient integration of several fundamental
algo-rithms, such as analytic energy gradients, geometry
optimi-zations for the relaxation of atomic positions within strained
and unstrained configurations, and CPHF/KS
self-consistent-field procedures. As for elastic, piezoelectric, and
photo-elastic constants, piezo-optic ones can also be decomposed
into purely electronic “clamped-ion” and nuclear
“internal-strain” contributions where the latter measures the piezo-optic
e↵ect due to the nuclear relaxation induced by strain,41,42
which is accounted for by optimizing the atomic positions
within the strained cell. Experimental measurements of the
static dielectric and piezo-optic response properties of
crys-tals should refer to the limit of infinite electric-field
wave-length . Practically, they are performed at finite values of ,
which are expected to correspond to sufficiently high
frequen-cies of the applied electric field to make nuclear
contribu-tions negligible, but not high enough for promoting electronic
excitations. These two constraints are such that the adopted
values of often do not correspond to the ! 1 limit of
the static CPHF/KS calculations. In the present
implementa-tion, we take advantage of recent developments on the
eval-uation of “dynamic” dielectric properties of solids31,43,44 _{to}
explicitly investigate the e↵ect of on computed piezo-optic
constants.

The resulting algorithm can be sketched as follows: (i) the starting crystal structure is fully optimized at the selected level of theory; (ii) cell gradients are computed on the optimized unstrained configuration as well as the equilibrium dielectric tensor (which is then inverted) with the CPHF/KS scheme (by default =1); (iii) a full symmetry analysis is performed in order to determine the non-null independent elastic and piezo-optic constants. The minimal set of independent deformations to be applied, out of a maximum of six, is also found; (iv) a given deformation is selected and the corresponding residual symmetry determined; for each deformation, Nsstrained configurations are defined according to a strain amplitude a (by default, Ns=2, corresponding to one “expanded” and one “contracted” configuration with a strain amplitude a = 0.015, i.e., a deformation of 1.5%

with respect to the unstrained lattice); (v) for each strained configuration, atomic positions are relaxed (default option) or not depending on whether one wants to go beyond or not the “clamped-ion” approximation; cell gradients and dielectric tensor of the strained configurations are computed; (vi) cell gradients and inverse dielectric tensors along a given deformation are fitted with singular-value-decomposition routines, their derivatives determined numerically and the corresponding elastic and photo-elastic constants obtained; (vii) once all independent deformations have been consid-ered and all independent elastic and photo-elastic constants determined, full elastic and photo-elastic tensors are built based on the symmetry analysis performed at the beginning, the elastic tensor is inverted and the piezo-optic constants obtained by combining the photo-elastic with the compliance tensors.

**C. Computational setup**

The algorithm described in Section II B has been
implemented into a development version of the Crystal14
program,31 _{which adopts a basis set of localized }
Gaussian-type functions (GTF). An all-electron basis set has been
adopted for describing O and Ca atoms, which consists
in a 6-31G(2d) contraction and a 6-31G(d) contraction of
GTFs, respectively. The large-core e↵ective pseudo-potential
derived by Hay and Wadt has been chosen for tungsten, which
leaves only the 5d and 6sp valence electrons to be
explic-itly described. A split-valence basis set has been adopted,
composed of two independent, single Gaussian sp shells, and a
3-1G contraction for d electrons.45_{Four di↵erent formulations}
of exchange-correlation DFT functional are considered: the
local-density approximation (LDA), SVWN functional,46,47
the generalized-gradient approximation (GGA), PBE48_{}
func-tional, and hybrid B3LYP49_{and PBE0}50_{functionals. }
Thresh-olds controlling the accuracy of Coulomb and exchange series
are set to 8, 8, 8, 8, 16.32_{Reciprocal space is sampled using}
a Monkhorst-Pack mesh with a shrinking factor of 6 for the
primitive cell of CaWO4, corresponding to 36 independent
k-points in the irreducible portion of the Brillouin zone.
A pruned grid with 1454 radial and 99 angular points is
used to calculate the DFT exchange-correlation contribution
through numerical integration of the electron density over the
unit cell volume.32 _{The self-consistent field convergence on}
energy was set to a value of 10 8 _{hartree for all geometry}
optimizations.

**III. RESULTS AND DISCUSSION**

Before discussing stress- or strain-induced anisotropic
re-sponses (elasticity, photo-elasticity, piezo-optics) of calcium
tungstate, CaWO4, we briefly comment on the description
provided by di↵erent classes of DFT functionals of
equilib-rium structural, elastic, electronic, and dielectric properties.
TableIreports such properties as computed with four
func-tionals (SVWN, PBE, B3LYP, and PBE0), belonging to three
rungs of “Jacob’s ladder,” along with their experimental
coun-terparts. Experimental values for lattice parameters a and c,
and fractional coordinates (x, y, z) of the oxygen atom in
gen-eral position are taken from the single-crystal X-ray study by
Hazen et al.51_{Voigt’s upper bound to the bulk modulus K}

V is defined in terms of the elastic constants as

KV =1

9[2C11+C33+2(C12+2C13)]. (12)
The experimental value reported in the table (89.4 GPa) refers
to 0 K and has been derived from the extrapolated elastic
constants measured in the temperature range 4.2–300 K by
Farley and Saunders;52_{note that computed values also refer}
to 0 K but neglect zero-point motion e↵ects which, on the
con-trary, are included in the experimental counterpart. Ordinary no
and extraordinary nerefractive indices, and the corresponding
birefringence =ne no are taken from Bond53 and from
Houston et al.54_{and correspond to an electric field wavelength}
=2500 nm, while theoretical values refer to the ! 1 limit
(see below for a theoretical investigation of the dispersion of
refractive indices with ).

From inspection of TableI, it is seen that, as expected, the simple LDA functional significantly underestimates the cell size (a by 1.6% and c by 1.4%), overestimates the bulk modulus (by almost 20 GPa, corresponding to about 22%), describes a relatively narrow electronic band gap of 3.6 eV (here a reliable experimental reference is not available), and largely overestimates the birefringence (by more than a factor of 2). The generalized-gradient PBE functional pro-vides a slightly better description of the lattice parameters, underestimating a by 0.4% and overestimating c by 2%, a similar description of the electronic band-gap (3.7 eV) but significantly improves upon LDA in the description of the bulk modulus (with an underestimation of about 4.5%) and of the birefringence. Hybrid functionals provide the best overall description of all considered properties, with PBE0 slightly outperforming B3LYP. Indeed, PBE0 gives an excel-lent description of the a lattice parameter (with a deviation TABLE I. Lattice parameters a and c (in Å), fractional coordinates (x, y, z) of the oxygen atom in general

position, Voigt bulk modulus KV (in GPa), electronic band gap Eg (in eV), ordinary noand extraordinary

nerefractive indices, and birefringence of CaWO4. Computed values, as obtained with four functionals, are

compared with experimental data from Refs.51–54.

a c x y z KV Eg no ne SVWN 5.158 11.210 0.237 0.093 0.038 108.6 3.6 1.878 1.908 0.030 PBE 5.221 11.660 0.239 0.103 0.041 85.2 3.7 1.806 1.823 0.017 B3LYP 5.277 11.649 0.236 0.105 0.042 86.1 5.8 1.725 1.732 0.007 PBE0 5.241 11.516 0.236 0.102 0.041 90.4 6.2 1.736 1.747 0.011 Expt. 5.243 11.374 0.241 0.099 0.039 89.4 . . . 1.872 1.885 0.013

smaller than 0.04%), only slightly overestimating the c one (by
1.2%), reliably describes the optical anisotropy of the system
(with a of 0.011 with respect to the experimental value of
0.013) and provides an excellent description of the elasticity
of the system, with a bulk modulus of 90.4 GPa with respect
to the experimental value of 89.4 GPa; an overestimation by
about 1% is perfectly compatible with the reduction of the
bulk modulus that would be induced by the neglected
zero-point motion and that could be evaluated by quasi-harmonic
calculations.55–59 _{As expected, hybrid functionals describe a}
significantly larger gap Eg (5.8–6.2 eV) than local-density
and generalized-gradient approximations. All functional give
a good description of the atomic positions within the cell.

**A. The elastic response**

As recalled in Section II A, a prerequisite to a reliable
description of the piezo-optics of a crystal is a good calculation
of its anisotropic elastic response. In Table II, we report the
seven symmetry-independent elastic sti↵ness Cvuand
compli-ance Svuconstants of tetragonal CaWO4. The shape of the full
fourth-rank elastic tensor for this system is given in
Equa-tion (5). In the table, the elastic constants are reported as
computed with four DFT functionals and compared with two
experimental determinations (one at room temperature and one
extrapolated down to 0 K from data collected in the 4.2–300 K
temperature range).52_{As expected from the overall structural}
description given in Table I, the LDA functional is seen to
systematically overestimate the Cvuand underestimate the Svu
constants. The PBE generalized-gradient functional tends to
slightly underestimate the elastic sti↵ness constants Cvuwhile
hybrid functionals (more so PBE0 than B3LYP) do provide a
satisfactory description of low-temperature elastic constants.
As the experimental piezo-optic constants were measured at
room temperature, it is interesting to illustrate the e↵ect of
temperature on the measured elastic constants. From
inspec-tion of the table, we can see that passing from 0 K to 300 K the
absolute values of all Cvuconstants are systematically reduced
by about 4% (a converse increase of about 4% of Svuconstants
is observed).

A better insight into the description provided by di↵erent DFT functionals of the anisotropy of the elastic response of a crystal can be achieved by analyzing directional elastic properties, such as directional seismic wave velocities (i.e., the velocities with which elastic waves do propagate within a crystal along di↵erent crystallographic directions). From a

fundamental point of view, within the elastic continuum model, the velocity of propagation of a seismic wave traveling along any general crystallographic direction represented by unit wave-vector ˆq, can be obtained from the elastic tensor via Christo↵el’s equation, which can be given an eigenvalues/ eigenvectors form as follows:8,60

Aqˆ_{U = V}2_{U} _{with} _{A}qˆ
j k=
1
⇢
X
il
ˆqiCi j k lˆql, (13)
where Aqˆ_{j k}is Christo↵el’s matrix, ⇢ the crystal density, i, j, k,l
=x, y, z represent Cartesian directions, ˆqi is the ith element
of the unit vector ˆq, V is a 3 ⇥ 3 diagonal matrix whose three
elements give the acoustic velocities, and U = (ˆu1,uˆ2,uˆ3) is
the eigenvector 3 ⇥ 3 matrix where each column represents
the polarization ˆu of the corresponding eigenvalue. The three
acoustic wave velocities, also referred to as seismic velocities,
can be labeled as quasi-longitudinal vp, slow quasi-transverse
vs1, and fast quasi-transverse vs2, depending on the polarization
direction ˆu with respect to wave-vector ˆq.61_{From directional}
seismic wave velocities, fundamental aspects of the elastic
anisotropy of a crystal, such as shear-wave birefringence and
azimuthal anisotropy, can be fruitfully discussed. These data
are reported in Figure1as computed with the four DFT
func-tionals. We observe that: (i) the four functionals provide a
similar overall description of the directional elastic properties
of CaWO4; (ii) the crystallographic direction of maximum
longitudinal propagation velocity is found between the [110]
and the [010] ones while the minimum longitudinal velocity
is along the [001] direction; (iii) the direction of maximum
propagation velocity of transverse waves is found between
the [100] and [110] ones while the minimum is between the
[110] and [010] ones; (iv) the basal ab plane is found to be
more anisotropic than the vertical ac plane; (v) LDA provides
the largest anisotropy, B3LYP the smallest while PBE and
PBE0 give a similar and intermediate description of the elastic
anisotropy.

**B. Photo-elastic and piezo-optic responses**

We can now compare theoretically calculated with exper-imentally determined stress-optical ⇡vuand strain-optical pvu constants of calcium tungstate. However, before doing so, it is worth illustrating how these two sets of data are obtained

• theoretically, strain-optical (photo-elastic) constants are determined as numerical derivatives of the inverse TABLE II. Symmetry-independent elastic sti↵ness Cvuand compliance Svuconstants of tetragonal CaWO4, as computed with four di↵erent DFT functionals

and compared to experimental data from Farley and Saunders52_{as measured at 300 K and extrapolated to 0 K.}

Elastic sti↵ness constants (GPa) Elastic compliance constants (Br ⌘ TPa1_{)}

C11 C12 C13 C33 C44 C66 C16 S11 S12 S13 S33 S44 S66 S16 SVWN 185.68 86.03 68.08 161.85 51.60 59.45 20.29 8.16 3.50 1.96 7.83 19.38 19.54 3.98 PBE 150.19 63.74 53.71 124.03 41.60 49.57 13.77 9.33 3.36 2.59 10.30 24.04 22.13 3.52 B3LYP 156.67 60.90 52.39 131.40 44.27 51.78 13.07 8.45 2.76 2.27 9.42 22.59 20.74 2.83 PBE0 161.65 67.05 54.68 137.67 45.63 54.17 15.85 8.56 3.16 2.14 8.97 21.91 20.46 3.43 Expt. 0 K 150.62 65.89 59.06 135.67 35.58 47.75 17.22 9.94 3.89 2.64 9.67 28.11 24.54 4.99 Expt. 300 K 143.87 63.50 56.17 130.18 33.61 45.07 16.35 10.45 4.15 2.71 10.02 29.75 26.03 5.30

FIG. 1. Directional seismic wave velocities of tetragonal CaWO4as

com-puted with four di↵erent DFT functionals.

of the dielectric tensor with respect to an applied strain according to Equation(7). Stress-optical constants are then obtained through the computed elastic compliance constants (⇡ =p S);

• experimentally, mechanical stresses are measured on
five di↵erently cut samples;18 _{previously }
experimen-tally determined elastic compliances52 _{S}

vuand
refrac-tive indices62 _{n}

o and ne are then used to solve a set of equations that provide stress-optical ⇡vu constants. Strain-optical constants are determined by combin-ing these stress-optical constants with the elastic

sti↵ness ones Cvupreviously experimentally measured (p = ⇡ C).

Let us stress that if on the one hand the theoretical
deter-mination of pvu and ⇡vu constants is achieved with a single
calculation within a homogeneous computational setup, on
the other hand experimental determinations of such properties
require a rather complex combination of measurements of
di↵erent quantities (mechanical stresses, elastic constants,
refractive indices) on di↵erent samples, which are generally
performed in di↵erent studies, by di↵erent groups, in di↵erent
conditions, and, above all, with di↵erent accuracies. Bearing
these considerations in mind, in Table IIIwe report the ten
symmetry-independent strain- and stress-optical constants (see
Equation(11)for the shape of the fourth-rankp and ⇡ tensors)
as computed with the four DFT functionals and as compared
with available experimental determinations. The full set of
piezo-optic ⇡vuconstants has recently been reported by Mytsyk
et al.18_{where just the sign of the ⇡}

61constant could not be
deter-mined while its absolute value was reported to be ⇡61=|0.16|
Br. Demyanyshyn et al.13 _{have then coupled such constants}
to the elastic sti↵ness ones to determine the photo-elastic pvu
constants: due to the uncertainty on the sign of the ⇡61constant,
two photo-elastic constants, p61 and p66, were not uniquely
determined (for ⇡61= 0.16 Br they got p61= 0.001 and
p66= 0.018, while for ⇡61= +0.16 Br they obtained p61
=0.025 and p_{66}= 0.031).

Regarding the e↵ect of DFT functional on such computed properties, from TableIIIwe see that: (i) the computed values of pvuconstants obtained with all functionals are rather consis-tent with each other, particularly so if generalized-gradient (PBE) and hybrid (B3LYP and PBE0) functionals are consid-ered (LDA providing slightly deviating results for some con-stants, such as p12, p13, p16, and p66); (ii) a similar trend is also observed for ⇡vuconstants where LDA deviates more from the other functionals due to its poorer description of the elastic TABLE III. Photoelastic pvu and piezo-optic ⇡vu symmetry-independent constants of CaWO4 as computed

with four di↵erent DFT functionals and as experimentally determined by Mytsyk and co-workers (see text for
details).13,17–19_{Depending on the sign of the ⇡}

61constant (experimentally ill-determined), di↵erent

experimen-tal values of p61and p66are found (values in parentheses correspond to ⇡61= 0.16 Br while the others to
⇡61=0.16 Br).
Photoelastic constants
p11 p12 p13 p31 p33 p44 p45 p16 p61 p66
SVWN 0.154 0.150 0.263 0.254 0.201 0.018 0.018 0.051 0.029 0.071
PBE 0.157 0.175 0.249 0.256 0.226 0.018 0.017 0.022 0.026 0.058
B3LYP 0.152 0.194 0.240 0.264 0.208 0.009 0.017 0.019 0.026 0.050
PBE0 0.177 0.185 0.255 0.265 0.229 0.014 0.019 0.032 0.025 0.055
Expt. 0.40 0.02 0.24 0.25 0.21 0.011 0.06 0.27 0.025 0.031
( 0.001) ( 0.018)
Piezo-optic constants (Br ⌘ TPa 1_{)}

⇡11 ⇡12 ⇡13 ⇡31 ⇡33 ⇡44 ⇡45 ⇡16 ⇡61 ⇡66 SVWN 0.417 0.035 1.467 0.788 0.578 0.352 0.345 1.006 0.058 1.151 PBE 0.308 0.387 1.706 0.946 1.001 0.436 0.404 0.430 0.128 1.104 B3LYP 0.256 0.622 1.480 1.030 0.759 0.202 0.384 0.283 0.149 0.896 PBE0 0.495 0.367 1.508 0.938 0.922 0.318 0.409 0.637 0.100 0.964 Expt. 1.86 0.60 1.52 1.02 1.01 0.33 1.77 5.64 |0.16| 0.63

compliance constants; furthermore, given the di↵erent descrip-tion of elastic constants provided by PBE, B3LYP, and PBE0, larger di↵erences (never exceeding a factor of 2.2 in the worst cases, though) are found on predicted piezo-optic constants by these functionals; (iii) given the overall better description of elastic constants (see Table II) and refractive indices (see TableI), hybrid functionals are expected to constitute the best choice for the calculation of these properties and to provide the most reliable results.

In order to compare computed constants with experimen-tally derived ones, let us group the 10 symmetry-independent components of both the photo-elastic and piezo-optic tensors into two sub-sets: a first sub-set contains the x13, x31,x33,x44, x61, and x66constants while the second sub-set contains the x11, x12, x45, and x16 ones, where x can be either p or ⇡. For the first sub-set, which contains 6 constants, consider-ing how delicate both the calculation and the experimental determination of these constants are, the agreement between computed and experimental values is very satisfactory, partic-ularly so if hybrid functionals are considered, as expected. Such a good agreement is a strong evidence of the accuracy of both the experimental reconstruction of these constants and the automated computational strategy here devised. Present calculations allow for the ambiguous determination of the sign of the ⇡61constant, which is indeed found to be positive by all functionals. Furthermore we find that by taking the posi-tive sign of this constant, the experimental values of the p61 (0.025) and p66( 0.031) constants are also found to be in much better agreement with present calculations. The small residual deviations between computed and experimental constants for this set might be due to either the neglect of thermal e↵ects on computed elastic properties (which, however, is expected to be rather small: about 4% as noticed above) or the finite value of the electric-field wavelength used in the experiments versus the = 1 of the calculations (see SectionIII Cfor an explicit investigation of such e↵ect).

The situation is completely di↵erent when the second sub-set of 4 constants is considered. In this case, indeed, there is little agreement between computed and experimentally derived values, with very large di↵erences on both absolute values and signs. Given that all computed constants are obtained with the same numerical accuracy, we have to deduce that the experimental reconstruction of these four constants is not as reliable as it was for the other six. On the contrary, present calculations do provide a complete, homogeneous set of all of the ten symmetry-independent photo-elastic and piezo-optic constants of CaWO4.

**C. Effect of the electric field wavelength**

As mentioned at the end of SectionIII B, experimental measurements of optical properties of crystals are performed using a finite value of the wavelength of the electric field, whereas theoretical calculations generally refer to the = 1 case. For instance, all of the experimental photo-elastic and piezo-optic constants of calcium tungstate reported in TableIII correspond to = 633 nm. One might wonder if some of the discrepancies between computed and experimentally derived constants could be ascribed to such an issue. Electric field

FIG. 2. Dependence on electric field wavelength of computed photo-elastic pvuand piezo-optic ⇡vuconstants of CaWO4. The dashed vertical lines

mark the experimental wavelength ( = 633 nm) used in the determination of the constants reported in TableIII. Values obtained with the PBE functional. Computed values for = 1 are represented by full circles.

frequency dependent optical properties of crystals can be
computed with a “dynamical” formulation of the CPHF/KS
approach.31,43,44_{The present algorithm for the calculation of}
photo-elastic and piezo-optic tensors has been generalized to
such a case too. In Figure2, we report computed pvuand ⇡vu
constants of CaWO4(just at the PBE level as similar trends
are observed also for other functionals) as a function of in
the range 500–1500 nm (continuous lines) while static values
obtained at = 1 are given as full circles. A dashed vertical
line marks the =633 nm value. We can clearly see that
the dispersion of all computed stress-optical and strain-optical
constants with is relatively small (i.e., their values change by
just few percents passing from = 1 to 633 nm). As regards
photo-elastic constants, p11and p12show the largest dispersion,
followed by p31and p66while the other constants are almost
flat. Piezo-optic constants show a slightly larger dispersion,
⇡66 exhibiting the largest among them. Overall, given the
small variations of all constants, the electric field frequency
dispersion can be ruled out as a possible reason for the large
inconsistency of computed and experimental constants of the
second sub-set discussed in SectionIII B.

**IV. CONCLUSIONS**

A computational strategy has been devised and imple-mented in a fully automated fashion for the quantum-mechani-cal prediction of piezo-optic fourth-rank tensors of crystals belonging to any space group of symmetry. This strategy is based on the simultaneous determination of elastic and photo-elastic tensors. A Coupled-Perturbed-Hartree-Fock/Kohn-Sham approach is used to compute the dielectric tensor of strained and unstrained configurations both in the static (infi-nite electric field wavelength) and dynamic (fi(infi-nite wavelength) cases. Both point and translation symmetries are fully ex-ploited thus drastically reducing the number of independent

components to be determined and the computational cost of all steps of the calculation.

The scheme has been applied to the CaWO4 calcium tungstate crystal and the full set of 10 symmetry-independent photo-elastic and piezo-optic constants has been determined using four di↵erent formulations of the exchange-correlation functional within the density-functional-theory. Present results validate a sub-set of 6 experimentally reconstructed symmetry-independent constants (x13,x31,x33,x44,x61, and x66, being x either the photo-elastic tensor p or the piezo-optic tensor ⇡) and provide more reliable values for a second sub-set of 4 constants (x11, x12, x45, and x16).

1_{J. F. Nye, Physical Properties of Crystals (Oxford University Press, Oxford,}

1957).

2_{H.-J. Weber,}_{Phys. Rev. B}_{51, 12209 (1995).}

3_{O. Krupych, V. Savaryn, A. Krupych, I. Klymiv, and R. Vlokh,}_{Appl. Opt.}

52, 4054 (2013).

4_{T. S. Narasimhamurty, Photoelastic and Electrooptic Properties of Crystals}

(Plenum, 1981).

5_{I. Slezinger, A. Alievskaya, and Y. Mironov,}_{Meas. Tech.}_{28, 1059 (1985).}
6_{J. Badoz, M. Billardon, J. C. Canit, and M. F. Russel,}_{J. Opt.} _{8, 373}

(1977).

7_{J. C. Kemp, J. Opt. Soc. Am.}_{59, 950 (1969).}

8_{B. A. Auld, Acoustic Fields and Waves in Solids (Krieger Publishing }

Com-pany, Malabar, Florida, 1973).

9_{J. Xu and R. Stroud, Acousto-Optic Devices: Principles, Design, and }

Appli-cations (Wiley, 1992).

10_{A. S. Andrushchak, B. G. Mytsyk, H. P. Laba, O. V. Yurkevych, I. M. Solskii,}

A. V. Kityk, and B. Sahraoui,J. Appl. Phys.106, 073510 (2009).

11_{B. G. Mytsyk, A. S. Andrushchak, N. M. Demyanyshyn, Y. P. Kost’, A. V.}

Kityk, P. Mandracci, and W. Schranz,Appl. Opt.48, 1904 (2009).

12_{A. Andrushchak, Y. Bobitski, M. Kaidan, B. Mytsyk, A. Kityk, and W.}

Schranz,Opt. Laser Technol.37, 319 (2005).

13_{N. M. Demyanyshyn, B. G. Mytsyk, Y. P. Kost, I. M. Solskii, and O. M.}

Sakharuk,Appl. Opt.54, 2347 (2015).

14_{H. Z. Cummins and P. E. Schoen, in Laser Handbook, edited by F. T. Arecchi}

and E. O. Schulz-Dubois (North-Holland Publishing Company, Amsterdam, 1972), p. 1029.

15_{D. Landheer, H. E. Jackson, R. A. McLaren, and B. P. Stoiche↵,}_{Phys. Rev.}

B13, 888 (1976).

16_{O. Krupych, V. Savaryn, and R. Vlokh,}_{Appl. Opt.}_{53, B1 (2014).}
17_{B. Mytsyk, N. Demyanyshyn, A. Andrushchak, Y. Kost’, O. Parasyuk, and}

A. Kityk,Opt. Mater.33, 26 (2010).

18_{B. Mytsyk, Ya. P. Kost’, N. Demyanyshyn, A. Andrushchak, and I. Solskii,}

Crystallogr. Rep.60, 130 (2015).

19_{B. Mytsyk, Y. Kost, N. Demyanyshyn, V. Gaba, and O. Sakharuk,}_{Opt. Mater.}

39, 69 (2015).

20_{R. Dovesi,}_{Int. J. Quantum Chem.}_{29, 1755 (1986).}

21_{C. Zicovich-Wilson and R. Dovesi,}_{Int. J. Quantum Chem.}_{67, 299 (1998).}
22_{C. Zicovich-Wilson and R. Dovesi,}_{Int. J. Quantum Chem.}_{67, 311 (1998).}
23_{R. Orlando, M. D. L. Pierre, C. M. Zicovich-Wilson, A. Erba, and R. Dovesi,}

J. Chem. Phys.141, 104108 (2014).

24_{K. Doll, N. M. Harrison, and V. R. Saunders,}_{Int. J. Quantum Chem.}_{82, 1}

(2001).

25_{K. Doll,}_{Comput. Phys. Commun.}_{137, 74 (2001).}

26_{K. Doll, R. Dovesi, and R. Orlando,}_{Theor. Chem. Acc.}_{112, 394 (2004).}
27_{K. Doll, R. Dovesi, and R. Orlando,}_{Theor. Chem. Acc.}_{115, 354 (2006).}

28_{M. Ferrero, M. Rérat, R. Orlando, and R. Dovesi,}_{J. Comput. Chem.}_{29, 1450}

(2008).

29_{M. Ferrero, M. Rérat, R. Orlando, and R. Dovesi,}_{J. Chem. Phys.}_{128, 014110}

(2008).

30_{M. Ferrero, M. Rérat, B. Kirtman, and R. Dovesi,}_{J. Chem. Phys.} _{129,}

244110 (2008).

31_{R. Dovesi, R. Orlando, A. Erba, C. M. Zicovich-Wilson, B. Civalleri, S.}

Casassa, L. Maschio, M. Ferrabone, M. De La Pierre, Ph. D’Arco et al.,Int. J. Quantum Chem.114, 1287 (2014).

32_{R. Dovesi, V. R. Saunders, C. Roetti, R. Orlando, C. M. Zicovich-Wilson, F.}

Pascale, K. Doll, N. M. Harrison, B. Civalleri, I. J. Bush et al., CRYSTAL14 User’s Manual, Università di Torino, Torino, 2014, http://www.crystal. unito.it.

33_{A. Erba, A. Mahmoud, R. Orlando, and R. Dovesi,}_{Phys. Chem. Miner.}_{41,}

151 (2014).

34_{A. Erba, A. Mahmoud, D. Belmonte, and R. Dovesi,}_{J. Chem. Phys.}_{140,}

124703 (2014).

35_{A. Erba, K. E. El-Kelany, M. Ferrero, I. Baraille, and M. Rérat,}_{Phys. Rev.}

B88, 035102 (2013).

36_{K. E. El-Kelany, P. Carbonnière, A. Erba, and M. Rérat,}_{J. Phys. Chem. C}

119, 8966 (2015).

37_{A. Erba, M. Ferrabone, J. Baima, R. Orlando, M. Rérat, and R. Dovesi,}

J. Chem. Phys.138, 054906 (2013).

38_{A. Erba and R. Dovesi,}_{Phys. Rev. B}_{88, 045121 (2013).}
39_{J. P. Perdew and K. Schmidt,}_{AIP Conf. Proc.}_{577, 1 (2001).}

40_{W. F. Perger, J. Criswell, B. Civalleri, and R. Dovesi,} _{Comput. Phys.}

Commun.180, 1753 (2009).

41_{G. Saghi-Szabo, R. E. Cohen, and H. Krakauer,}_{Phys. Rev. Lett.}_{80, 4321}

(1998).

42_{A. Dal Corso, M. Posternak, R. Resta, and A. Baldereschi,}_{Phys. Rev. B}_{50,}

10715 (1994).

43_{L. Bernasconi, S. Tomi´c, M. Ferrero, M. Rérat, R. Orlando, R. Dovesi, and}

N. M. Harrison,Phys. Rev. B83, 195325 (2011).

44_{A. Ferrari, R. Orlando, and M. Rérat,}_{J. Chem. Theor. Comput.} _{11(7),}

3245–3258 (2015).

45_{F. Corá, A. Patel, N. M. Harrison, R. Dovesi, and C. R. A. Catlow,}_{J. Am.}

Chem. Soc.118, 12174 (1996).

46_{J. C. Slater,}_{Phys. Rev.}_{81, 385 (1951).}

47_{S. H. Vosko, L. Wilk, and M. Nusair,}_{Can. J. Phys.}_{58, 1200 (1980).}
48_{J. P. Perdew, K. Burke, and M. Ernzerhof,}_{Phys. Rev. Lett.}_{77, 3865 (1996).}
49_{A. D. Becke,}_{J. Chem. Phys.}_{98, 5648 (1993).}

50_{C. Adamo and V. Barone,}_{J. Chem. Phys.}_{110, 6158 (1999).}

51_{R. M. Hazen, L. W. Finger, and J. W. Mariathasan,}_{J. Phys. Chem. Solids}_{46,}

253 (1985).

52_{J. Farley and G. Saunders,}_{Solid State Commun.}_{9, 965 (1971).}
53_{W. L. Bond,}_{J. Appl. Phys.}_{36, 1674 (1965).}

54_{T. W. Houston, L. F. Johnson, P. Kisliuk, and D. J. Walsh,}_{J. Opt. Soc. Am.}

53, 1286 (1963).

55_{A. Erba,}_{J. Chem. Phys.}_{141, 124115 (2014).}

56_{A. Erba, M. Shahrokhi, R. Moradian, and R. Dovesi,}_{J. Chem. Phys.}_{142,}

044114 (2015).

57_{A. Erba, J. Maul, R. Demichelis, and R. Dovesi,}_{Phys. Chem. Chem. Phys.}

17, 11670 (2015).

58_{A. Erba, J. Maul, M. De La Pierre, and R. Dovesi,}_{J. Chem. Phys.}_{142,}

204502 (2015).

59_{A. Erba, J. Maul, M. Itou, R. Dovesi, and Y. Sakurai,}_{Phys. Rev. Lett.}_{115,}

117402 (2015).

60_{M. J. P. Musgrave, Crystal Acoustics (Holden-Day, San Francisco, }

Califor-nia, 1970).

61_{B. B. Karki, L. Stixrude, and R. M. Wentzcovitch,}_{Rev. Geophys.}_{39, 507,}

doi:10.1029/2000RG000088 (2001).